Int J Thermophys (2011) 32:1210–1233 DOI 10.1007/s10765-011-1011-1

A Comparison of Surface Tension, Viscosity, and Density of Sn and Sn–Ag Alloys Using Different Measurement Techniques

Tomasz Gancarz · Zbigniew Moser · Władysław Ga˛sior · Janusz Pstru´s · Hani Henein

Received: 19 January 2010 / Accepted: 25 May 2011 / Published online: 11 June 2011 © The Author(s) 2011. This article is published with open access at Springerlink.com

Abstract This work is aimed at comparing several methods for the measurement of physical properties for molten Sn and Sn–Ag alloys, namely, surface tension, den- sity, and viscosity. The method used for viscosity in this work is the modiﬁed capillary method. For surface tension and density, the data used for comparison were previously measured using the maximum bubble pressure method and the dilatometer technique, respectively, for four Sn–Ag alloys having (3.8, 32, 55, and 68) at% Ag. The results are compared with those obtained using a new method based on a ﬂuid draining from a crucible under the inﬂuence of gravity, designated the Roach–Henein (RH) method. This new method enables the determination of these three physical properties in one set of measurements. Liquid Sn was used as well as two liquid Sn–Ag alloys having (3.8 and 34.6) at% Ag with the RH method. It was determined that the RH method may be used to simultaneously obtain surface tension, viscosity, and density and that the errors associated with these measurements were similar to those obtained using traditional and separate techniques. Comparisons of the measured viscosity and sur- face tension to those predicted using thermodynamic models will also be presented. Finally a comparison of mixing model predictions with the experimentally measured alloy surface tension and viscosity is also presented.

Keywords Capillary method · Density · Dilatometer method · Maximum bubble-pressure method · Molten tin · Molten tin–silver alloys · RH method · Surface tension · Viscosity

T. Gancarz (B) · Z. Moser · W. Ga˛sior · J. Pstru´s Institute of Metallurgy and Materials Science, Polish Academy of Sciences, Krakow, Poland e-mail: [email protected]

T. Gancarz · H. Henein Department of Chemical and Materials Engineering, University of Alberta, Edmonton, AB, Canada 123 Int J Thermophys (2011) 32:1210–1233 1211

List of Symbols A Molar surface area in a monolayer of species i, m2 Ao Pre-exponential in Eq. 39,mPa· s B Starting liquid height Hs in the reservoir, m Cm Cumulative mass, kg D(T ) Diameter of lower container in CM method as a function of temperature T,m G Free energy, J · mol−1 G∗ Activation energy of the alloy, J · mol−1 G Change in activation energy, J · mol−1 Hs Height of liquid at which measurement started, initial height, m Hf Height of liquid at which measurement ended, ﬁnal height, m Hm Average height, m H m Molar enthalpy of mixing for the liquid alloy, J · mol−1 L Constant set to 1.091 for liquid metals assuming close-packed structures M Molecular weight, kg · mol−1 −1 N0 Avogadro’s number, mol Ns Depth of capillary immersion at the beginning of measurement, m Nf Depth of capillary immersion at the end of measurement, m Nm Substitute depth of measurement, m 3 −1 Qexp Experimental volumetric ﬂow rate, m · s R Universal gas constant, J · mol−1 · K−1 S Area under the curve between Hs and Hf ,m· s T Temperature, K V Volume of draining ﬂuid, volume liquid, m3 3 Vi Molar volume of pure liquid i, m 3 Vs Volume of liquid drawn into the reservoir at the start of measurement, m V E Excess molar volume of alloy components Wi, j Interaction coefﬁcient for binary alloys X Mole fraction, dimensionless Z Coordination number a Polynomial constant describing slope of the discharge coefﬁcient curve, dimensionless b Polynomial constant describing the y-intercept of the discharge coefﬁcient curve, dimensionless g Acceleration of gravity, m · s−2 h Planck’s constant, J · s hexp Liquid head above a point of reference in RH method, m l Length of capillary, m p Pressure difference, Pa r Capillary radius in MC method, m rc Crucible radius, m ro Oriﬁce radius in RH method, m t Time, s u Velocity, m · s−1

123 1212 Int J Thermophys (2011) 32:1210–1233

α Constant β Parameter corresponding to the ratio of the coordination number in the surface phase to that in the bulk phase (Z S/Z B) η Viscosity, mPa · s ηH Hagenbach correction for viscosity, mPa · s ρ Density, kg · m−3 σ Surface tension, mN · m−1 Diameter of the bottom tank (crucible), m ρgr0hexp Bo Bond number σ , dimensionless Cd Discharge coefﬁcient, dimensionless 2 /( π 3) Fr Froude number (Qexp 2 gro ), dimensionless ρ Q Re Reynolds number 2 exp , dimensionless πr0η

Superscripts BBulk E Excess S Surface ex Excess

Subscripts Ag Silver Sn Tin

1 Introduction

Over the past few years, efforts have been underway worldwide to eliminate lead from solders due to its toxicity. In proposing a new lead-free solder material, several physi- cal properties must be evaluated including the liquid density, viscosity, and gas–liquid surface tension as a function of temperature. In previous studies carried out by Moser et al. [1] on tin and liquid Sn–Ag alloys, the surface tension was measured using the maximum bubble-pressure method, the den- sity was determined using the dilatometric technique, and the viscosity was reported using the capillary method that was previously used by Ga˛sior et al. [2] on Pb–Sn alloys. Roach and Henein [3,4] have developed a new method enabling the simulta- neous measurement of surface tension, viscosity, and density in one run for ﬂuids, herein referred to as the RH method. The method is based on a ﬂuid exiting a crucible as a stream ﬂowing under gravity. The model developed can be used to calculate these physical properties from only one experiment at a desired temperature. It was reported in Roach and Henein [4,5] that for liquid Al, the values of surface tension and density are reasonable, but the value of the viscosity differed from published values by nearly an order of magnitude. It was hypothesized that this may have been due to the fact that in the gravity ﬂow method, the ﬂuid ﬂow is under turbulent conditions; therefore, the measured viscosity may be related to a turbulent dynamic viscosity. Hence, 123 Int J Thermophys (2011) 32:1210–1233 1213 the values obtained were much lower than those reported by Rothwell [6] and by Kisun’ko et al. [7]. It was, therefore, decided to undertake parallel measurements of viscosity on tin and tin–silver alloys and to carry out a comparison of the surface tension and density with previously published measurements by Moser et al. [1]. Such a comparison of measurements will also provide a broader base of experimental results to compare against thermodynamic models of the physical properties of these alloys. This would also enable the extension of the data available in the SURDAT database [8].

2 Viscosity Measurements: Modiﬁed Capillary (MC) Method

The measurement of viscosity is based on the Hagen-Poisseulle (H-P) formula of cap- illary ﬂow, which states that the volume of liquid ﬂowing under laminar conditions out of a capillary is inversely proportional to the viscosity of the ﬂuid and the capil- lary length but directly proportional to the pressure difference between the end of the capillary and the surface of the liquid in the reservoir as well as to the radius of the capillary raised to the fourth power:

V πpr4 = (1) t 8ηl where V is the liquid volume (m3) that ﬂows out during time t (s), p is the pressure difference (Pa), r is the capillary radius (m), η is the viscosity (mPa · s), and l is the capillary length (m). The viscosity can be calculated by rearranging Eq. 1 as shown in

πr 4t η = p (2) 8lV

Thus, if V, t, and p are measured in an experiment, the Hagen-Poisseulle law in the form of Eq. 2 may be applied to obtain η. However, this only applies in the case when the liquid ﬂows out from the capillary induced by a constant difference in pressure p between the end of the capillary and the surface of the liquid in the reservoir. This is the case when the pressure is significantly higher than the hydrostatic pressure in the reservoir. In the case of free outﬂow of liquid induced by a changing hydrostatic pressure (the lowering height of liquid column H in the reservoir) both the volume, V , and pressure difference, p, are functions of time. Thus, V = V (t), p = p(t), and H = H(t) are all functions of time and Eq. 1 takes the following form:

dV (t) πr 4 = p (t) (3) dt 8ηl 1 123 1214 Int J Thermophys (2011) 32:1210–1233

Fig. 1 Schematic of capillary ﬂow method for measuring viscosity

Since the hydrostatic pressure changes with the height of the liquid column, H(t), in the reservoir (Fig. 1), Eq. 3 can be expressed in the following form:

π R2dH(t) πr 4ρg = H(t) (4) dt 8ηl

Multiplying both sides of Eq. 4 by dt and dividing by H(t), π, and R2, the following equation is obtained:

dH(t) ρgr4 = dt (5) H(t) 8ηlR2

Deﬁning α, a constant, to be given by,

ρgr4 α = . (6) 8ηlR2 123 Int J Thermophys (2011) 32:1210–1233 1215

Eq. 5 can be re-written as

dH(t) = αdt (7) H(t)

Integrating Eq. 7 over the limits H = Hs at t = 0 and H = Hf at t = t as shown in

Hf t dH(t) = αdt (8) H(t) Hs 0 yields

H ln f =−αt (9) Hs

Rearranging Eq. 9,

Hf = Hs exp(−αt) (10) which can be used to calculate the height of the liquid in the reservoir after time t (Fig. 1). Hence, after measuring the time of outﬂow of different volumes from the reservoir through the capillary, and assuming the parameter α of Eq. 10, the viscosity can be calculated from Eq. 6. The experiment is carried out in such a way, that during time, t, the outﬂow of a particular liquid volume is contained between heights Hs and Hf of the reservoir (Fig. 1). Hm is the average height of liquid represented by the change of height from Hs to Hf during time t and can be calculated as an area S under the curve given by Eq. 10 divided by the time of liquid outﬂow t. S, then, can be expressed as the following integral:

t H H S = H (−αt) t =− s −αt − s s exp d α e α (11) 0

After dividing by t, the average height, Hm, is given by S H −α H = = s 1 − e t (12) m t αt

Incorporating Eqs. 9 and 10 into Eq. 12, the average height, Hm, can be calculated from the initial height, Hs (t = 0) and ﬁnal height, Hf (t = t) as follows:

(Hs − Hf ) Hm = (13) lnHs − lnHf 123 1216 Int J Thermophys (2011) 32:1210–1233

Thus, the liquid volume V that ﬂows into the bottom under a changing hydrostatic pressure p1(t) may be written as

(Hs − Hf ) p1 = ρg (14) lnHs − lnHf

Taking into consideration the Hagenbach correction ηH [9] of the kinetic energy decrease of the liquid stream, which can be calculated from the following formula:

Vρ η =− (15) H 8πlt and substituting Eq. 14 into Eq. 2, the following equation is obtained: πr 4tρg (H − H ) Vρ η = s f − (16) 8lV (lnHs − lnHf ) 8πlt

Thus, the viscosity of the liquid with density ρ can be calculated. Note that from the experiment, the time, t, of the outﬂow of liquid volume, V (contained between heights Hs and Hf ) through the capillary of radius, r, and length, l, must be measured. Before starting the experiment, liquid is induced into the capillary and reservoir with the aid of a vacuum pump. Thus, the height of the liquid in the bottom tank will increase over the duration of the experiment. A correction of the pressure change p2(t) connected with the increase of liquid level in the bottom tank, into which the liquid from the reservoir ﬂows must be incorporated into the model. The change of pressure p2(t) can be expressed according to a similar analysis presented above:

Ns − Nf p2 = ρg (17) lnNs − lnNf in which N is the depth of capillary immersion before the suction of liquid up to the 2 reservoir (m), Ns = Vs/(πΦ /4) is the depth of capillary immersion at the beginning of the measurement, e.g., after the suction of liquid of volume V into the reservoir (t = 0) (m), Nf = N − Ns is the depth of capillary immersion at the end of the experiment (m), i.e., after the ﬂow of the liquid of volume V, Vs is the volume of liquid drawn into the reservoir (m3), Φ is the diameter of the bottom tank (crucible) (m) (Fig. 1),

−βt N(t) = N − Nse (18) where

β =−1/t ln Ns/N (19) and Hs − Hf Ns − Nf p = p1 − p2 = ρg − (20) lnHs − lnHf lnNs − lnNf 123 Int J Thermophys (2011) 32:1210–1233 1217

Thus, Eq. 20 represents the pressure change brought about by the level of liquid in the bottom tank changing due to drawing in of liquid from the capillary. This is valid provided that the volume of liquid leaving the reservoir of diameter 2R and entering the bottom tank of diameter Φ are the same. Then the increase of the liquid level height in time t may be expressed as a ratio of the volume of liquid which arrives into the bottom tank divided by its area. This leads to the relationship describing the change of immersion of the capillary (depth) in time t of the outﬂow of liquid followed with the substitution with an average value Nm given by 2 2 Nm = N − 4Vs/πΦ + (2R/Φ) (21) in which the depth Ns at the beginning of the measurement (m) is

2 Ns = N − 4Vs/πΦ (22)

Vs is the volume of liquid sucked into the reservoir at the start of the measurement 3 (m ), Φ is the diameter of the bottom tank (m), and Nm is the substitute depth of measurement (m). Finally, the pressure difference p, which is used in Eq. 1, can be calculated from the formula, Φ2 − 4r 2 H − H 4V p = ρg c s f − N + s 2 2 (23) Φ lnHs − lnHf πΦ

The derived relations were tested by measuring the viscosity of carbon tetrachlo- ride, methyl alcohol, and mercury. The measurements of liquid height changes in the reservoir after time t are recorded and the results are shown in Fig. 2.

Fig. 2 Height of liquid in the 70 capillary as a function of time HS for different liquids in the modiﬁed capillary (MC) method 60

50

40 ht, cm g

HM Hei 30

20 HF Hg CCl4 CH3OH H2O 10 0 100 200 300 400 500 Time, s 123 1218 Int J Thermophys (2011) 32:1210–1233

Fig. 3 Experimental results of viscosity versus literature data from Iida and Guthrie [10]

They fully conﬁrm the above relation, which describes the liquid column height in the reservoir after time t, because each curve can be represented with an equation of the general form,

−α H(t) = Be t (24) where B is a starting liquid height Hs in the reservoir (Fig. 1). The viscosity can be determined using Eq. 6 and the measured α parameter. The measurement results for the mentioned earlier liquids, except for mercury, are presented in Fig. 3 (crosses) in ref- erence to literature data (full line) [10]. Very good agreement between experimentally determined viscosity data and that published in the literature is seen in Fig. 3.Note that the derived relations apply only for the case of laminar ﬂow of liquid through the capillary, i.e., for a Reynolds number Re < 2300, inﬂuenced by hydrostatic pressure. The Reynolds number in the experiments oscillated in the range of 1600 to 2000. For the case of mercury, the viscosity value was obtained with a high error because it had a much higher Reynolds number (turbulent outﬂow), and thus it was not included in the plot (Fig. 3). Before the start of the experiment with a metal or alloy, it was placed in the bot- tom tank, a graphite crucible, above which the reservoir with the capillary of known dimensions was installed. Both elements were positioned in an alundum tube with a wound coil. Next, the device was hermetically sealed, air pumped out from the exper- imental space, and then it was back-ﬁlled with a protective atmosphere (mixture of argon and hydrogen). The protective atmosphere was passed through the apparatus during heating for several hours. In turn, using a micrometer screw, the lower crucible was lifted until it met the bottom of the capillary, which resulted in a fast increase of the gas pressure ﬂowing out of the capillary. The capillary was then immersed to a speciﬁed depth, and the apparatus was thermally equilibrated for an hour. Next the 123 Int J Thermophys (2011) 32:1210–1233 1219

Fig. 4 Viscosity of tin versus 2 temperature using MC method compared with average data Chhabra and Sheth from Chhabra and Sheth [11] (dashed line), and with Gebhardt s

et al. [12](solid line) .

a 1.6 , mP y

This study 1.2

Viscosit Gebhardt at al.

0.8 400 600 800 1000 1200 1400 Temperature, K

Fig. 5 Viscosity of liquid tin 3.5 and tin–silver alloys versus Ag-Sn temperature: solid circles Gebhardt et al. [12], stars MC 3 Gebh65Ag method

s .

a 2.5 Gebh52.3Ag mP

, Gebh26.8Ag y 2 SnAg68

1.5

Viscosit SnAg55.4

1 SnAg32 Sn-nowe GebhSn 0.5 400 800 1200 1600 Temperature, K

liquid (alloy) from the crucible was sucked up to the reservoir, and the measurement of the outﬂow time of the determined volume of liquid through the capillary could begin. Results of viscosity measurements as a function of temperature are plotted in Fig. 4 for Sn and in Fig. 5 for Sn–Ag alloys. Excellent agreement with literature data is observed [11,12]. The viscosity as a function of temperature is expressed by an Arrhe- nius equation, and the results are shown in Table 1. 123 1220 Int J Thermophys (2011) 32:1210–1233

Table 1 Temperature dependence of the viscosity of Sn and Sn–Ag alloys with associated errors using the MC method

E/(RT) XAg η = Ae η at 823 K (mPa · s) ∂η (mPa · s) ∂ A ∂ E AE

0, XSn = 1 0.497713 5411.2 1.132 ±0.044 ±0.057 ±341 0.038 0.463408 6160.8 1.181 ±0.072 ±0.0466 ±477 0.32 0.587148 7314.4 1.783 ±0.044 ±0.0415 ±339 0.55 0.557895 8974.4 2.180 ±0.123 ±0.0989 ±706 0.68 0.769598 10398.4 3.734 ±0.089 ±0.0469 ±350

3 Surface Tension, Density, and Viscosity Studies Using the RH Method

Roach and Henein [3–5] developed a new method for ﬂuids to simultaneously measure the surface tension, viscosity, and density in one experiment. The RH method is based on a ﬂuid exiting a crucible as a stream, ﬂowing under gravity. It was reported that for liquid Al the values of surface tension and density were reasonable [4], but the values of viscosity differed from published values (Rothwell [6] and Kisun’ko [7]) by nearly an order of magnitude. It was hypothesized that this may be due to the fact that since in the gravity ﬂow method, ﬂuid is under turbulent conditions, the Reynolds numbers are in excess of 4000, contrary to viscous ﬂow of the H-P law. The essential part of the experimental apparatus for measurements of surface ten- sion, viscosity, and density are described in detail in Roach and Henein [4]. It consists of a draining vessel depicting free gravitational ﬂow of a ﬂuid through an oriﬁce placed in the bottom of the crucible (Fig. 6).

Fig. 6 Schematic of draining vessel system depicting ﬂow rate of a ﬂuid through an oriﬁce placed at the bottom, the RH method

123 Int J Thermophys (2011) 32:1210–1233 1221

The derivation proposed by Roach and Henein [4] is similar to the traditional Ber- noulli formulation, except that an additional term is included because the pressure induced from the surface tension is quantiﬁed in the model. Therefore, the Froude and Bond numbers are analyzed. The Froude number represents the ratio of the inertial force of the stream to the potential force of the liquid head above the oriﬁce discharge. The Bond number represents the ratio of the potential force to the surface force of the stream exiting the oriﬁce. The following relation should be satisﬁed:

Fr + 1/Bo = 1 (25)

Starting from the known radius of the oriﬁce, r0, 0.001 m, the height for water varied from 0.08 m to 0.05 m, while for tin, it ranged from 0.05 m to 0.02 m which satisfy the relation between Fr and Bo [3–5]. The different heights for water and tin are due to differences in their densities and surface tensions. Using liquids of known physical properties and an oriﬁce of a given diameter to be used with melts, a calibration of Cd versus Re was developed. Water and tin were used as calibration ﬂuids with their physical properties taken from the literature [13–16]. During the ﬂow, the mass was measured as a function of time using a load cell. The cumulative mass Cm versus time curve for tin and water is obtained and ﬁtted with a third-order polynomial. An example of the polynomial for tin at 723 K is given by the following equation and a sample result is shown in Fig. 7: −8 3 −5 2 Cm =− 6 × 10 t − 3 × 10 t + 0.12t + 0.011 (26)

3 −1 Knowing Cm, the experimental volumetric ﬂow rate, Qexp (m · s ) can be deter- mined,

1 ∂C Q = m (27) exp ρ ∂t

Fig. 7 Cumulative mass Cm as a function of time for tin at 723 K through a 0.001 m radius of the oriﬁce 123 1222 Int J Thermophys (2011) 32:1210–1233

The discharge coefﬁcient, Cd, of the oriﬁce which characterizes friction losses in the oriﬁce, is determined and is deﬁned as the ratio between the experimental ﬂow 3 −1 rate Qexp and theoretical ﬂow rate Qtheor (m · s ). It is given by

Qexp Cd = (28) σ πr 2 2g h − 0 exp ρgr0

Qexp is also used to calculate the Reynolds number (Re). The Reynolds number is used in characterizing the inertial forces relative to viscous losses in the oriﬁce, and is calculated using the relation,

2ρ Qexp Reexp = (29) πr0η

Finally, the relation of Cd versus Re is plotted and is shown in Fig. 8. Six different calibration curves are shown in Fig. 8. Four of them are for tin at varying temperatures and two for water also at different temperatures. Clearly, the friction losses (Cd)in the oriﬁce are nearly the same in all cases. For materials of unknown properties, the relation between Cd and Re will be used to determine the physical properties. This will be discussed later. A third-order polynomial was used to ﬁt all six data sets and is expressed as

−12 3 −8 2 Cd = 2 × 10 Re − 4 × 10 Re + 0.0003Re − 0.0114 (30)

In this work only the data with Re > 4000 were used in determining the physical properties of tin and Sn–Ag alloys. A linear ﬁt to the Cd versus Re calibration data for Re > 4000 is therefore used and is given by

0.8

0.7

0.6

0.5 water 333 K water 353 K d 0.4 C tin 723 K 0.3 tin 773 K 0.2 tin 823 K 0.1 tin 873 K

0 0 1000 2000 3000 4000 5000 6000 7000 Re Fig. 8 Calibration for a 0.002 m diameter oriﬁce and height of 0.06 m to 0.08 m using water at 333 K and 353 K, and tin for a height of 0.004 m to 0.06 m at 723 K, 773 K, 823 K, and 873 K 123 Int J Thermophys (2011) 32:1210–1233 1223

−5 Cd = 5 × 10 Re + 0.6844 (31)

Using data determined in the calibration procedure along with Eq. 28, the calcu- lations of the surface tension, density, and viscosity were undertaken by an iterative method.

3.1 Surface Tension

The method for determining the physical properties of Sn and Sn–Ag alloys is based on the following equation:

⎡ ⎤ 2 1 Qexp σ = ρgr ⎣h − ⎦ (32) 0 exp ( + ) π 2 2g aRe b r0 by means of an iterative method with initial values of the density of tin with coefﬁ- cients a and b taken from Eq. 31. In this section, the results obtained for the surface tension will be discussed. Subsequently, the results for the density and viscosity will be presented. The results for tin are shown in Fig. 9, and those for Sn–Ag alloys for the surface tension as a function of temperature are presented in Table 2 and plotted in Fig. 10. With an increase in temperature, the surface tension of liquid Sn decreases linearly. The results show very good agreement with the values calculated with the equation (A) recommended by Keene [17], over the whole range of temperature. Also, good agreement is observed between our data and the results of Fiori from Ref. [14]atlow

Fig. 9 Surface tension of pure tin as a function of temperature compared with literature data: triangles Fiori [13], stars Tanaka [13], diamonds (A) using σ = 613.6 − 0.103T Keene [17], squares Mills and Su [13], cross Leeetal.[18], open circles Gasior et al. [2], and closed circles this work (RH method) 123 1224 Int J Thermophys (2011) 32:1210–1233

Table 2 Relations for surface tension of Sn and Sn–Ag alloys with errors using the RH method

−1 −1 XSn σ = A + BT σ at 823 K (mN · m ) ∂σ (mN · m ) ∂ A ∂ B AB

1.000 623.7 −0.1173 527.4 ±8.0 ±41.6 ±0.0504 0.962 625.5 −0.1100 534.9 ±10.5 ±20.2 ±0.0261 0.654 638.5 −0.0720 579.2 ±11.3 ±18.4 ±0.0193

Fig. 10 Surface tension of Sn and Sn–Ag alloys as a function of temperature using the RH method compared with literature data of Gasior et al. [2], Moser et al. [1], and Kucharski and Fima [19] temperature, and the results from Lee et al. [18] at high temperature. The results of Ga˛sior et al. [2] and Tanaka from Ref. [14] are slightly lower compared with our data. The results for Sn and Sn–Ag alloys using the RH method are plotted in Fig. 10. With increasing temperature, the surface tension of liquid Sn and Sn–Ag alloys decreases linearly. One can see that the surface-tension temperature coefﬁcients (dσ/dT )for eutectic compositions determined by the RH method and by Moser et al. [1] are very similar. From Fig. 10 it is shown that good agreement is observed between the RH method results and literature data [1,2,19]; also evident in Fig. 10 is that the surface tension increases with the concentration of silver.

3.2 Modeling of the Surface Tension

Surface-tension data for seven Ag–Sn alloys from a previous study [1] were interpreted by the Butler model [20] using the following equation: − S RT 1 xSn 1 ex S S ex B B σ = σAg + ln + G T, X − G T, X A 1 − xB A Ag Sn Sn Sn Ag Sn Ag X S = σ + RT Sn + 1 E,S , S − E,B , B Sn ln B GSn T XSn GSn T XSn (33) ASn XSn ASn 123 Int J Thermophys (2011) 32:1210–1233 1225

−1 −1 where R is the gas constant in J · mol · K ; T is the temperature in K; σAg and σSn −1 are the surface tensions of pure silver and tin in mN·m ; Ai is the molar surface area ( = 2 S B in a monolayer of pure liquid i i Ag or Sn) in m ; and XSn and XSn are the mole fractions of Sn in the surface and the bulk phase, respectively. The molar surface area Ai can be obtained from the relation,

= 1/3 2/3 Ai LN0 V0 (34)

3 where N0 is the Avogadro number; Vi is the molar volume of pure liquid i (m ); L is E,S( , ) usually set to 1.091 for liquid metals assuming close-packed structures; Gi T Xi E,B( , ) and Gi T Xi are the partial excess Gibbs energies of component i in the surface and bulk phases as function of T and Xi , with Xi being the mole fraction of component i (J · mol−1). The following equation provides a relation for the excess Gibbs energy in the bulk and surface phases: E,S , S = β E,B , S Gi T Xi Gi T Xi (35) where β is a parameter corresponding to the ratio of the coordination number in the surface phase to that in the bulk phase Z S/Z B, and it is assumed that β = 0.83 for liquid metals [21]. The surface tension of liquid Ag–Sn alloys was calculated using the values of the partial excess Gibbs energies of Ag and Sn from optimized thermodynamic parame- ters [22]. For calculations of molar volumes of Ag–Sn alloys, the densities determined from this study were used with densities for pure Ag from [23] and for pure tin from [24]. The excess free energy was calculated using a binary model. This model for binary solutions is given by

2 3 ex G = Xi X j Wi, j (36) i=1 j=2 where Wi, j is the interaction coefﬁcient for binary alloys which is obtained from the database of thermodynamic properties by ADAMIS [25]: WAg,Sn = (−4902.5 − 4.30532T ) + (−16474 + 3.12507T ) XAg − XSn 2 −7298.6 XAg − XSn (37)

Xi ’s are the mole fractions. Surface-tension data for pure liquid Sn and Ag were taken from [26] and [27]. Figure 11 illustrates a comparison between the results of calcu- lations (lines) and the experimental data (circle, square) for respective compositions. The surface tension calculated from the model decreases with increasing temperature and increases with increasing Sn concentration, which is in accordance with experi- mental results. Good agreement is observed between calculated and all experimental data. 123 1226 Int J Thermophys (2011) 32:1210–1233

Fig. 11 Surface tension of tin and Sn–Ag alloys as a function of temperature compared with 1000 Ag-Sn the Butler model: solid line -1

circles m Butler model, Gasior et . al. [2], squares this work (RH 623 K method) mN 800 1273 K ce Tension, a 600 rf u S

400 0.0 0.2 0.4 0.6 0.8 1.0

XSn

3.3 Density

The results for the density of tin and Sn–Ag alloys that were calculated simultaneously with the surface tension using Eq. 32 and associated errors are reported in Table 3. The maximum error in the data is less than 2.5 %. Data from Table 3 for tin were used to prepare Fig. 12. With increasing tempera- ture, the density of liquid Sn decreases linearly. The results obtained show very good agreement with the results of Berthou and Tougas [28] and Pstrus [29] over the whole range of temperature. Also, good agreement is observed between the data obtained using the RH method and the results of Smithells [30] and Kucharski [24]. The Sn–Ag alloy density is also shown in Fig. 13 together with a comparison with other literature data. The results in Fig. 13 indicate that with increasing temperature, the density of liquid Sn and Sn–Ag alloys decreases linearly. One can see that the density temperature coefﬁcients (dρ/dT ) for eutectic compositions determined by using the RH method and by Moser et al. [1] and Kaban et al. [31] are very similar. From Fig. 13 it is noted that good agreement is observed between data obtained using the RH method and literature data; and also, the density increases with increasing concentration of silver.

Table 3 Relations for density of Sn and Sn–Ag alloys with errors using the RH method

−3 −3 XSn ρ = A + BT ρ at 823 K (kg · m ) ∂ρ (kg · m ) ∂ A ∂ B

AB

1.000 7.2986 −0.000648 6.765 ±0.018 ±0.092 ±0.000112 0.962 7.3793 −0.000591 6.893 ±0.030 ±0.058 ±0.000075 0.654 8.6433 −0.001094 7.743 ±0.193 ±0.314 ±0.000330

123 Int J Thermophys (2011) 32:1210–1233 1227

Berthou 6900 Kucharski_1977 Kucharski_2005 6850 Pstrus_PhD Smithells -3 6800 This work

6750

6700 Density, kg·m

6650

6600 680 730 780 830 880 930 Temperature, K Fig. 12 Density of pure tin as a function of temperature compared with literature data of Kucharski_1977 Kucharski [24], Kucharski_2005 Kucharski and Fima [19], Berthou Berthou and Tougas [28], Pstrus_PhD Pstru´s[29], Smithells Smithells [30], diamonds this work (RH method)

Fig. 13 Density of Sn and Sn–Ag alloys as a function of temperature using the RH method compared with literature data of Moser et al. [1], Kaban et al. [31], and Berthou and Tougas [28]

3.4 Viscosity

Finally the values of the viscosity of Sn and Sn–Ag alloys were also calculated from Eq. 32 which was used to determine the density and surface tension using the RH method. They are presented in Table 4 and used in plotting Fig. 14. Data from Gebhardt et al. [12] are also plotted in Fig. 14. 123 1228 Int J Thermophys (2011) 32:1210–1233

Table 4 Relations for viscosity of Sn and Sn–Ag alloys with errors using the RH method

E/(RT) XSn η = Ae η at 823 K (mPa · s) ∂η (mPa · s) ∂ A ∂ E

AE

1.000 0.3847256 7511.66 1.153 ±0.013 ±0.059 ±348 0.962 0.3935107 7791.64 1.229 ±0.110 ±0.067 ±647 0.654 0.5799891 7821.34 1.820 ±0.097 ±0.079 ±493

Fig. 14 Viscosity of tin and 2.4 Sn–Ag alloys as a function of temperature using the RH SnAg34.6 SnAg3.8 method (diamonds) compared with points from Gebhardt et al. 2

[12] s . a 1.6 mP , y

1.2 Sn SnAg52.3 Viscosit SnAg26.8 0.8 Sn

0.4 400 800 1200 1600 Temperature, K

The resulting viscosity data were interpreted using an Arrhenius equation. With increasing temperature, the viscosity of liquid Sn and Sn–Ag alloys decreases log- arithmically. One can see that the viscosity temperature coefﬁcients (dη/dT ) for Sn and for Sn–Ag compositions determined by the RH method and by Gebhardt et al. [12] are very similar. The results for viscosity measurements for Sn and Sn–Ag alloys using the MC and RH methods are shown in Fig. 15 and Table 4. The results from both methods are clearly in agreement with each other.

3.5 Modeling of Metal Alloy Viscosity Based on Thermodynamic and Physical Properties

The scientiﬁc literature provides models for predicting the viscosity of liquid alloys using thermodynamic properties such as the excess molar free energy or the molar enthalpy of mixing as well as, in some cases, using physical prop- erties such as the viscosity of components, density, or molar volume of alloys, atomic masses and radii. The earliest and simplest equation (Eq. 40) was derived by Moelwyn-Hughes and reported in [32]: 123 Int J Thermophys (2011) 32:1210–1233 1229

Fig. 15 Viscosity as a function 3.5 of temperature from MC method (open and ﬁlled stars), from RH method (diamonds) and from 3 Gasior et al. [2](crosses) s

. SnAg34.6

a 2.5 P SnAg68 SnAg3.8 2

1.5 Viscosity, m SnAg55 Sn 1 SnAg3.8 SnAg32 Sn 0.5 400 600 800 1000 1200 1400 Temperature, K

H m η = (η X + η X ) 1 − 2 (38) 1 1 2 2 RT

For a binary system, η, η1, and η2 denote the viscosity of an alloy and its compo- nents; X1, X2 represent the molar fractions of the components; R is the gas constant; T is the temperature, and H m is the molar enthalpy of mixing for the liquid alloy. In the case of multicomponent alloys, the authors have applied a simple extension of Eq. 38 taking the second part of the expression as a constant, while the ﬁrst relation was substituted with a sum of three products ηi Xi . In 1987, Sichen et al. [33] proposed the following equations, which comprised the thermodynamic properties of liquid solutions, their densities, activation energies, and viscosities of components, to calculate the viscosity of multicomponent solutions:

G∗ η = A exp (39) o RT hN ρ A = 0 (40) o M n n−1 n ∗ = ∗ + + G Xi Gi RT Xi Xk G (41) i=1 i=1 k=i+1 where G∗ denotes the activation energy of the alloy, G is the change of activation ∗ ∗ energy, T is the temperature, G1 and G2 are activation energies of the components, R is the gas constant, ρ is the alloy density, N0 is the Avogadro number, h is Planck’s constant, and M is the atomic mass of alloy components. 123 1230 Int J Thermophys (2011) 32:1210–1233

In the same year, Seetharaman and Sichen [34] modiﬁed the relationship describing the activation energies into the following form:

n n−1 n ∗ = ∗ + + G Xi Gi 3RT Xi Xk G (42) i=1 i=1 k=i+1

The authors of the report presented the calculations of both approaches; as it fol- lows from their observations, the application of Eqs. 41 and 42 does not always give results that are in agreement with experimental data. The model of Kozlov–Romanov–Petrov [35] also applies the mixing enthalpy of liquid solutions for the prediction of the viscosity, similar to the Moelwyn-Hughes model. It is represented with the following logarithmic equation:

n H m ln (η) = Xi ln(ηi ) − (43) 3RT i=1

A transformation of Eq. 43 gives the following expression, which describes the vis- cosity of alloys in the form of an exponential function: n H m η = exp Xi ln(ηi ) − (44) 3RT i=1

In Eqs. 43 and 44, the viscosity of an alloy and its components is denoted by η and ηi , mole fractions of components by Xi , the temperature by T , and the gas constant by R. In 2004, Kaptay [36] proposed a modiﬁcation of the Seetharaman and Sichen model (Eq. 42) for viscosity calculations; it consists of substituting the excess free energy into the equation of activation energy with the enthalpy of mixing multiplied by an α coefﬁcient, which, according to the author, amounts to 0.155 to 0.015, resulting in the following equation for the viscosity with the following form: n ∗ m hN = Xi G − αH η = 0 exp i 1 i (45) n + E i=1 Xi Vi V RT

All the symbols in Eq. 45 have the same meaning as in the earlier presented models E (Eqs. 38 to 44), while the new quantities, Vi and V , refer to the molar volume of alloy components and the excess molar volume of an n-component alloy. It should be noted that the molar volume included in the denominator of Eq. 45 is identical with the M/ρ expression from the Seetharaman–Sichen model. The presented models of viscosity calculations based on the thermodynamic prop- erties were applied for the binary Sn–Ag alloys for the same concentrations of metals such as those examined with the method of capillary ﬂow and the RH technique. The equations describing the dependence of the viscosity on temperature applied in the calculations are reported in Table 5. 123 Int J Thermophys (2011) 32:1210–1233 1231

Table 5 Dependences of the Metal η = Aexp(E /RT)(mPa · s) Author viscosity of liquid metals Ag and a Sn on temperature Ag 0.5976exp(19137/(RT)) Gebhardt et al. [12] Sn 0.4993exp(5675/(RT)) This work

In the case of Sn, the equation presented was derived based on three series of data: from the examination of the Pb–Sn system [2], from the measurements using the MC method, and from the measurements using the RH method. The temperature depen- dences of the Ag viscosity were studied based on the values measured by Gebhardt et al. [12]. The excess free energy was calculated using the binary model as were the calculations of surface tension and Wi, j . The enthalpy of mixing applied in Eqs. 38, 44, and 45 was calculated from the following equation: dGex H m = Gex + T − (46) dT p

The thermodynamical parameters, describing binary interaction coefﬁcients WAg,Sn are the same as in Eq. 37, and the viscosities of pure Sn and Ag are presented in Table 5. Modeling of the viscosity of Ag–Sn alloys was conducted using ﬁve models and presented in Fig. 16. The lack of a universal model and the difﬁculty in modeling the viscosity are apparent. The best agreement between measured and calculated viscos- ity is given by the Seetharaman and Sichen model [34]. The data obtained from the Moelwyn-Hughes [32] model yield much higher values. One can notice that in the

15 Seetharaman_Du Sichen 14 Kozlow_Romanow_Petrow 13 Ag-Sn Sichen_Boygen_Seetharaman 12 T=823 K Moelwyn_Hughes 11 Kaptay s .

a 10 This work: MC method 9 This work: RH method mP ,

y 8 7 6

Viscosit 5 4 3 2 1 0 0.2 0.4 0.6 0.8 1

XSn Fig. 16 Comparison of viscosity with models: Seetharaman and Du Sichen [34], Kozlov et al. [35], Sichen et al. [33], Moelwyn-Hughes [32], Kaptay [36], and this work: diamonds MC method, inverted triangle RH method 123 1232 Int J Thermophys (2011) 32:1210–1233

Moelwyn-Hughes [32] model only the enthalpy of mixing is used for calculation of the viscosity and for such a case for alloys with a negative value of Hm. The calculated E viscosity will always be higher than that for the ideal solution (G and Hm = 0); and for alloys with a positive value of Hm, the viscosity will be lower than that for ideal solutions.

4 Summary

Calculations of the surface tension, density, and viscosity performed recently using the RH method were compared with those measured by using the MC method. A com- parison between viscosity results using the MC method and RH method are presented. The values are in very good agreement, as is the case for density and surface tension from the RH method compared with previously published data of Ga˛sior et al. [2]. It is surprising that using a seemingly simple procedure of gravity ﬂow from a crucible, one instrument/run generates values for three physical properties with good accuracy. It should be noted that the ﬂow of ﬂuid draining from a crucible in the RH method and analyzed here were for Re > 4000. Experiments carried out using cap- illary ﬂow were laminar with Re < 2000. The RH method shows great promise to efﬁciently generate physical property data of alloys. The measured results of surface tension show excellent agreement with the Butler model. For viscosity, the thermodynamic model proposed by Seetharaman and Sichen is in agreement with the experimental measurements of both the MC and RH methods.

Acknowledgments The authors wish to acknowledge the Natural Science and Engineering Research Council for funding the experimental work and analysis of the Edmonton effort. The authors from IMIM PAS wish to thank the Ministry of Science and Higher Education for ﬁnancing the project on enlarging the SURDAT database.

Open Access This article is distributed under the terms of the Creative Commons Attribution Noncom- mercial License which permits any noncommercial use, distribution, and reproduction in any medium, provided the original author(s) and source are credited.

References

1. Z. Moser, W. Ga˛sior, J. Pstru´s, J. Phase Equilib. 22, 254 (2001) 2. W. Ga˛sior, Z. Moser, J. Pstru´s, M. Kucharski, Arch. Metall. 46, 23 (2001) 3. S.J. Roach, H. Henein, Can. Metall. Quart. 42, 175 (2003) 4. S.J. Roach, H. Henein, Metall. Mater. Trans. B 36, 667 (2005) 5. H. Henein, Can. Metall. Quart. 44, 261 (2004) 6. E. Rothwell, J. Inst. Met. 90, 389 (1962) 7. V.Z. Kisun’ko, I.A. Novokhatskii, A.Z. Beloborodov, Y.B. Bychkov, A.I. Pogorelov, Tsvetnte Metally (Non-Ferrous) 24, 84 (1983) 8. Z. Moser, W. Ga˛sior, A. De˛bski, J. Pstru´s, Database of Lead-free Soldering Materials (Institute of Metallurgy and Materials Science PAS, Krakow, 2007), ISBN 83-60768-01-3 9. E.E. Schpilrajn, W.A. Fomin, S.N. Scovorodko, G.F. Sokol, Isledowanie Wiazkosti Zidkich Meta- lov (Moskwa, Nauka, 1983) 10. T. Iida, R.I.L. Guthrie, The Physical Properties of Liquid Metals (Clarendon Press, Oxford, 1988), p. 77 11. R. Chhabra, D. Sheth, Z. Metallkd. 81, 264 (1990) 12. E. Gebhardt, M. Becker, E. Tragner, Z. Metallkd. 46, 379 (1955) 123 Int J Thermophys (2011) 32:1210–1233 1233

13. K.C. Mills, Y.C. Su, Int. Mater. Rev. 51, 329 (2006) 14. D.R. Lide (ed.), CRC Handbook of Chemistry and Physics, 88th edn. (CRC Press, Boca Raton, FL, 2007) 15. R.R. Miller, Liquid Metals Handbook (Atomic Energy Commission and the Department of Navy, Washington, DC, 1952) 16. B.B. Alchagirov, A.M. Chochaeva, High Temp. 38, 44 (2000) 17. B.J. Keene, Int. Mater. Rev. 38, 157 (1993) 18. J. Lee, W. Shimoda, T. Tanaka, Mater. Trans. 45, 2864 (2004) 19. M. Kucharski, P. Fima, Monasch. Chem. 136, 1841 (2005) 20. J.A.V. Butler, Proc. R. Soc. Lond., Ser. A CXXXV, 348 (1932) 21. T. Tanaka, K. Hack, T. Iida, S. Hara, Z. Metallkd. 87, 380 (1996) 22. I. Ohnuma, X.J. Liu, K. Ishida, J. Electron. Mater. 28, 1164 (1998) 23. I. Ohnuma, X.J. Liu, Y.Inohana, K. Ishida, Z. Moser, W. Ga˛sior, J. Pstru´s, W. Zakulski, in Proceedings of CALPHAD XXIX (Massachusetts Institute of Technology, Cambridge, MA, 2000), p. 15 24. M. Kucharski, Arch. Hut. 22, 181 (1977) 25. H. Ohtani, M. Miyashita, K. Ishida, J. Jpn. Inst. Met. 63, 685 (1999) 26. W. Ga˛sior, Z. Moser, J. Pstru´s, J. Phase Equilib. 24, 504 (2003) 27. W. Ga˛sior, J. Pstru´s, Z. Moser, A. Krzyz˙ak, K. Fitzner, J. Phase Equilib. 24, 40 (2003) 28. P.E. Berthou, R. Tougas, Metall. Trans. 1, 2978 (1970) 29. J. Pstru´s, Physico-Chemical Properties of New Solder Alloys on Example of Sn-Zn-In System, Ph.D. Thesis, Krakow, 2008 30. W.F. Gale, T.C. Totemeier (eds.), Smithells Metals Reference Book (Elsevier, Butterworth-Heine- mann, Oxford, 2004) 31. I. Kaban, S. Mhiaoui, W. Hoyer, J.-G. Gasser, J. Phys.: Condens. Matter 17, 7867 (2005) 32. E.A. Moelwyn-Hughes, Phys. Chem. 434 (1970) 33. D. Sichen, J. Bygdén, S. Seetharaman, Metall. Mater. Trans. B 25, 519 (1994) 34. S. Seetharaman, D. Sichen, Metall. Mater. Trans. B 25, 589 (1994) 35. L.Y. Kozlov, L.M. Romanov, N.N. Petrov, Izv. Vuzov. Chernaya Metall. 3, 7 (1983) 36. G. Kaptay, in Proceeedings of MicroCAD 2003, International Conference Section: Metallurgy (University of Miskolc, Hungary, 2003), p. 23

123